Microwave-assisted large scale synthesis of lanthanide metal-organic frameworks (Ln-MOFs), having a preferred conformation and photoluminescence properties.
Bag, Partha Pratim; Wang, Xu-Sheng; Cao, Rong; Dalton transactions (Cambridge, England : 2003) 44 (2015) 11954–11962; doi:10.1039/c5dt01598g

data_7035254
_publ_section_title
;
 Microwave-assisted large scale synthesis of lanthanide metal-organic
 frameworks (Ln-MOFs), having a preferred conformation and
 photoluminescence properties.
;
_journal_issue                   26
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              11954
_journal_page_last               11962
_journal_paper_doi               10.1039/c5dt01598g
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'C30 H27 Cl N5 O14 Yb'
_chemical_formula_weight         890.06
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-03-10 deposited with the CCDC.
2015-05-26 downloaded from the CCDC.
;
_cell_angle_alpha                106.107(3)
_cell_angle_beta                 98.869(2)
_cell_angle_gamma                100.650(3)
_cell_formula_units_Z            2
_cell_length_a                   9.4951(3)
_cell_length_b                   12.5595(4)
_cell_length_c                   18.9191(6)
_cell_measurement_reflns_used    8857
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      73.56
_cell_measurement_theta_min      3.74
_cell_volume                     2079.23(12)
_computing_cell_refinement
'CrysAlisPro, Agilent Technologies, Version 1.171.37.33'
_computing_data_collection
'CrysAlisPro, Agilent Technologies, Version 1.171.37.33'
_computing_data_reduction
'CrysAlisPro, Agilent Technologies, Version 1.171.37.33'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Atlas'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0341
_diffrn_reflns_av_sigmaI/netI    0.0427
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            10762
_diffrn_reflns_theta_full        74.23
_diffrn_reflns_theta_max         74.23
_diffrn_reflns_theta_min         3.77
_exptl_absorpt_coefficient_mu    5.298
_exptl_absorpt_correction_T_max  0.875
_exptl_absorpt_correction_T_min  0.789
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'CrysAlisPro, Agilent Technologies, Version 1.171.37.33'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.422
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             882
_exptl_crystal_size_max          0.0563
_exptl_crystal_size_mid          0.0372
_exptl_crystal_size_min          0.0251
_platon_squeeze_details
;
;
_refine_diff_density_max         3.137
_refine_diff_density_min         -2.562
_refine_diff_density_rms         0.195
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     439
_refine_ls_number_reflns         7962
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.063
_refine_ls_R_factor_all          0.0660
_refine_ls_R_factor_gt           0.0632
_refine_ls_shift/su_max          0.005
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1124P)^2^+12.8534P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1816
_refine_ls_wR_factor_ref         0.1842
_reflns_number_gt                6872
_reflns_number_total             7962
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5dt01598g2.cif
_cod_data_source_block           yb_final
_cod_depositor_comments
'Adding full bibliography for 7035246--7035254.cif.'
_cod_original_cell_volume        2079.23(11)
_cod_database_code               7035254